The degree of reaction (α) of a silicon and silica mixture is equal to the sample weight loss
described by Equation 11, if all of the weight loss is due to the investigated reaction. Values
for weight loss as function of time and temperature (obtained by experiments) can therefor be
used to model the reactivity of a silicon and silica mixture. An Arrhenius relation has been used
to model the reactivity and the final equation is including the reaction area in addition to the
reaction constant and activation energy, as presented in Equation 13. The available reaction
area was assumed to be described by the initial area multiplied with the fraction unreacted
sample and an agglomeration factor, presented by Equation 14. The surface area of silicon was
used as initial reaction area due to the fact that initial surface area of silicon was lower than
initial surface area of silica. The agglomeration factor was included to take into account that
the reaction area decreases significantly when both phases are liquid, due to agglomeration. The
factor (F) is set to be equal to 1 below the melting point of quartz, and equal to 0.5 above it,
as described by Equation 15.
is the available reaction area,A_{0,Si} is the initial reaction area [cm^{2}·g^{−1}], F is the agglomeration
factor, Q is the activation energy [J/mol], R is the gas constant and T is the temperature [K].

The reaction constant and activation energy were obtained from experimental data by the use of an Arrhenius plot and linear regression. Equation 16 was obtained by integration of Equation 13, as described in Appendix I. The left side of the equation can be plotted based on experimental values, towards corresponding 1/T on the x-axis. This was done and a linear regression was used to find an equation that fits the points. The reaction constant is then equal to the exponential of the regression intersection with 1/T = 0 and the activation energy is equal to the slope of the regression multiplied by -R.

ln(−ln(1−α))−ln(A0,Si·F)−ln(t) =ln(k0)− Q

RT (16)

3.6.1 Probability and Statistics

Linear regression is used to fit the experimental data in an Arrhenius plot. The regression is
based on minimisation of the sum of square errors and the coefficient of determination (R^{2}) is
used as a measure of quality. One should be aware of the fact that R^{2} can be made artificially
high by an unwise practice of overfitting[41]. Additional terms in the model should only be
added it if it can be justified by an observed phenomena (eg. agglomeration of phases leading to
a significant decrease in reaction area above melting point of quartz) and should not be added
with the main goal of increasing the coefficient of determination.

A 95% prediction interval described by Equation 17 is used in this report to determine whether multiple types of quartz can be fitted to the same model. A group of 17 result (both from this master thesis and the specialisation project delivered by Sindland) from different experiments with one type of quartz (quartz A) was used to develop a linear regression and a prediction interval based on this population can than be created. It can be justified to include the future measurements in the same model, regardless of the raw materials used, if 95% of the new results lay within the prediction interval. In that case, where 95% of the new measurements lay within the prediction interval, a new regression can be obtained based on all of the data. One can say that there is a high probability that all of the raw materials have the same true linear regression.

This will be the method of determining whether reactivity of silicon and silica mixtures depend on the type of quartz used or not.

ˆ

### 4 Results

The weight loss of different silicon and quartz mixtures after isothermal heat treatment can be
correlated to the rate of the Si+SiO_{2} reaction and it is therefor the most important result
of this report. SEM and macro images have been obtained from each sample after heating, to
investigate the phase distribution and any reaction that might affect the correlation between
weight loss and reactivity. Additional investigation of each quartz sample have been performed
to be able to correlate any difference between them to difference in reactivity. That includes
investigation of phase distribution after heating at 1650°C for 120 minutes and wettability of
silicon on substrates made of each quarts type.

4.1 Weight loss

17 isothermal heat treatment experiments were performed as part of this thesis and the weight loss after heating is listed in Table 6 and shown in Figure 27. The weight loss increase expo-nentially with increasing temperature, even though the holding temperature has been decreased for experiments at higher temperatures. Five different types of quartz have been used in the experiments and the different types of quartz are indicated in Figure 28. There is no significant difference between the weight loss of the different quart samples.

Table 6: Quartz type, fraction, crucible temperature and holding time for each experiment is listed as well as sample weight loss after heating. Each sample was weighted to 20,0g prior to heating with a Si:SiO2 molar ratio of 1:1. The weight loss increase with temperature.

Quartz Fraction [mm] T [°C] thold [min] Weight loss [wt.%] Exp. Nr.

A 2-4,7 1670 120 3,25 M2

Figure 27: The weight loss after heating samples of quartz A to E mixed with silicon. The colour indicate the isothermal holding time. The dashed line is a regression based on all of the results.

Figure 28: The weight loss after heating samples of quartz A to E mixed with silicon. The colour indicate the type of quartz used in each experiment. The dashed line is a regression based on all of the results.